Total Energy Calculations¶
Calculation Details¶
We use density functional theory as implemented in the Vienna Ab Initio Simulation Package (VASP) software^{1} to evaluate the total energy of compounds. For the exchangecorrelational functional, we employ a mix of Generalized Gradient Approximation (GGA) and GGA+U, as described later in this manual. We use the Projector Augmented Wave (PAW) method for modeling core electrons with an energy cutoff of 520 eV. This cutoff corresponds to 1.3 times the highest cutoff recommended among all the pseudopotentials we use (more details can be found in the Pseudopotentials Choice manual). All calculations are performed at 0K and 0atm. All computations are performed with spin polarization on and with magnetic ions in a highspin ferromagnetic initialization (the system can of course relax to a low spin state during the DFT relaxation). We used a kpoint mesh of 1000/(number of atoms in the cell) for all computations, the MonkhorstPack method for the kpoint choices (but \(\Gamma\)centered for hexagonal cells) and the tetrahedron method to perform the kpoint integration. Pymatgen could change those default parameters if they are not adequate for the computation (e.g., switch to another kpoint integration scheme). Some details of our calculation method can be found in ref ^{2}; however, the Materials Project has updated many parameters as documented throughout the Methodology sections.
Crystal structures¶
We use input structures from the Inorganic Crystal Structure Database (ICSD),^{3} and relax all cell and atomic positions in our calculation two times in consecutive runs. When multiple crystal structures are present for a single chemical composition, we attempt to evaluate all unique structures as determined by an affine mapping technique.^{4}
Total energy convergence¶
We currently employ a kpoint mesh of 1000 per reciprocal atom (pra). We performed a convergence test of total energy with respect to kpoint density and convergence energy difference for a subset of chemically diverse compounds for a previous parameter set, which employed a smaller kpoint mesh of 500 pra. Using a 500 pra kpoint mesh, the numerical convergence for most compounds tested was within 5 meV/atom, and 96% of compounds tested were converged to within 15 meV/atom. Results for the new parameter set will be better due to the denser kpoint mesh employed. Convergence will depend on chemical system; for example, oxides were generally converged to less than 1 meV/atom.^{5}
Structure convergence¶
The energy difference for ionic convergence is set to 0.0005 * natoms in the cell. Data on expected accuracy on cell volumes can be found in a previous paper.^{2} We have found these parameters to yield wellconverged structures in most instances; however, if the structures are to be used for further calculations that require strictly converged atomic positions and cell parameters (e.g. elastic constants, phonon modes, etc.), we recommend that users reoptimize the structures with tighter cutoffs or in force convergence mode.
Total Energy Adjustments¶
To better model energies across diverse chemical spaces, we apply several adjustments to the total energy. These adjustments are described below.
Default corrections¶
Gases, liquids, and elements¶
Our total energy calculations are for periodic solids at 0K. For elements that are gaseous in their standard state, our raw calculations do not represent the same phase as standard experimental data. In addition, there may be GGA errors associated with reducing gas phases in gastosolid reactions. Rather than calculating the liquid/gas energies directly, we adjust the energies of several elements that are liquid or gaseous at room temperature using Wang's method.^{5} The besttested fit is for oxygen gas reacting to form to oxides. We have adjusted energies of the following compounds:
 $\ce{O2}$, $\ce{N2}$, $\ce{Cl2}$, $\ce{F2}$, $\ce{H2}$
The adjusted energies outside of $\ce{O2}$ are not as welltested, and calculations involving these elements should be taken with greater caution. For example, it is assumed in our elemental gas adjustments that reactions to the solid will involve reduction of the gas.
GGA+U calculations and adjustments to match GGA energies¶
Some compounds are better modeled with a U correction term to the density functional theory Hamiltonian while others are better modeled without (i.e., straight GGA). Energies from calculations with the +U correction are not directly comparable to those without. To obtain better accuracy across chemical systems, we use GGA when appropriate, GGA+U otherwise, and mix energies from the two calculation methodologies by adding an energy correction term to the GGA+U calculations to make them comparable to the GGA calculations. The idea behind this approach is to split reactions into subreactions that are wellmodeled by GGA, wellmodeled by GGA+U, or a binary formation reaction that can be estimated from known experimental data. More details on this method can be found in ref ^{6}.
Accuracy of Total Energies¶
To estimate the accuracy of our total energy calculations, we compute reaction data and compare against experimental data. Note that this data set was compiled using a lower kpoint mesh and pseudopotentials with fewer electrons than the current Materials Project parameter set.
Estimating errors in calculated reaction energies¶
The accuracy of calculated reaction energies depends on the chemical system investigated. In general, GGA calculations have similar errors among chemically similar systems. Hence, reaction energies between chemically similar systems (e.g., a reaction where the reactants and products are all oxides, such as $\ce{MgO + Al2O3 > MgAl2O4}$) tend to have smaller errors than reactions between chemically dissimilar systems (e.g., between metals and insulators).
Figure 1: Errors in Calculated Formation Energies for 413 binaries in the Kubaschewski Tables. Energies are normalized to per mol atom.
To provide a quantitative indicator of the error we may expect from the reaction calculator, we have computed the reaction energies of 413 binaries in the Kubaschewski Tables formed with Group V, VI and VII anions. Figure 1 shows the errors in the calculated formation energies (compared to the experimental values) for these compounds. The mean absolute error (MAE) is around 14 kJ mol$^{1}$. 75% of the calculated formation energies are within 20 kJ mol$^{1}$. We also found that compounds of certain elements tend to have larger errors. For example, Bi, Co, Pb, Eu, U, Tl and W compounds often have errors larger than 20 kJ mol$^{1}$.
It should be noted that while an MAE of 14 kJ mol$^{1}$ is significantly higher than the desired chemical accuracy of 4 kJ mol$^{1}$, it compares fairly well with the performance of most quantum chemistry calculations^{7}. Other than the most computationally expensive model chemistries such as G1G3 and CBS, the reaction energy errors of most computational chemistry model chemistries are well above 10 kJ mol$^{1}$.
For oxidation of the elements into binary compounds, an average error of ~4% or 33 kJ/mol$\ce{O2}$ is typical.^{8} For conventional ternary oxide formation from the elements, we have found a mean relative absolute error of about 2%.^{6}
Sources of error¶
The largest contribution to the error comes from the inability of the GGA to fully describe electronic exchange and correlation effects. In addition, there is some error associated with neglecting zeropoint effects and with comparing 0K, 0atm computations with roomtemperature enthalpy experiments. The latter effect was estimated to contribute less than 0.03 eV/atom by Lany.^{9} The stability of antiferromagnetic compounds may be underestimated, as the majority of our calculations are performed ferromagnetically only. The effect of magnetism may be small (under 10 meV/atom) or large (100 meV/atom or greater), depending on the compound. For compounds with heavy elements, relativistic effects may lead to greaterthanexpected errors.
GGA errors on reaction energies between chemically similar compounds¶
We recently conducted a more indepth study comparing GGA (+U) reaction energies of ternary oxides from binary oxides on 135 compounds. ^{10}
The main conclusions are:
 The error in reaction energies for the binary oxide to ternary oxides reaction energies are an order of magnitude lower than for the more often reported formation energies from the element. An error intrinsic to GGA (+U) is estimated to follow a normal distribution centered in zero (no systematic underestimation or overestimation) and with a standard deviation around 24 meV/at.
 When looking at phase stability (and for instance assessing if a phase is stable or not), the relevant reaction energies are most of the time not the formation energies from the elements but reaction energies from chemically similar compounds (e.g., two oxides forming a third oxide). Large cancelation of errors explain this observation.
 The +U is necessary for accurate description of the energetics evene when reactions do not involve change in formal oxidation states
Accuracy of Calculated Volumes¶
A discussion of errors in calculated volumes can be found in the Volume Change Error manual.
Citation¶
To cite the calculation methodology, please reference the following works:
 A. Jain, G. Hautier, C. Moore, S.P. Ong, C.C. Fischer, T. Mueller, K.A. Persson, G. Ceder., A HighThroughput Infrastructure for Density Functional Theory Calculations, Computational Materials Science, vol. 50, 2011, pp. 22952310. DOI:10.1016/j.commatsci.2011.02.023
 A. Jain, G. Hautier, S.P. Ong, C. Moore, C.C. Fischer, K.A. Persson, G. Ceder, Accurate Formation Enthalpies by Mixing GGA and GGA+U calculations, Physical Review B, vol. 84, 2011, p. 045115. DOI:10.1103/PhysRevB.84.045115
Authors¶
 Anubhav Jain
 Shyue Ping Ong
 Geoffroy Hautier
 Charles Moore
References¶

Kresse, G. & Furthmuller, J., 1996. Efficient iterative schemes for ab initio totalenergy calculations using a planewave basis set. Physical Review B, 54, pp.1116911186. ↩

A. Jain, G. Hautier, C. Moore, S.P. Ong, C.C. Fischer, T. Mueller, K.A. Persson, G. Ceder., A HighThroughput Infrastructure for Density Functional Theory Calculations, Computational Materials Science. vol. 50 (2011) 22952310. ↩↩

G. Bergerhoff, The inorganic crystalstructure database, Journal Of Chemical Information and Computer Sciences. 23 (1983) 6669. ↩

R. Hundt, J.C. SchÃ¶n, M. Jansen, CMPZ  an algorithm for the efficient comparison of periodic structures, Journal Of Applied Crystallography. 39 (2006) 616. ↩

L. Wang, T. Maxisch, G. Ceder, Oxidation energies of transition metal oxides within the GGA+U framework, Physical Review B. 73 (2006) 16. ↩↩

A. Jain, G. Hautier, S.P. Ong, C. Moore, C.C. Fischer, K.A. Persson, G. Ceder, Formation Enthalpies by Mixing GGA and GGA+U calculations, Physical Review B, vol. 84 (2011), 045115. ↩↩

J.B. Foresman, A.E. Frisch, Exploring Chemistry With Electronic Structure Methods: A Guide to Using Gaussian, Gaussian. (1996). ↩

A. Jain, S.a SeyedReihani, C.C. Fischer, D.J. Couling, G. Ceder, W.H. Green, Ab initio screening of metal sorbents for elemental mercury capture in syngas streams, Chemical Engineering Science. 65 (2010) 30253033. ↩

S. Lany, Semiconductor thermochemistry in density functional calculations, Physical Review B. 78 (2008) 18. ↩

G. Hautier, S.P. Ong, A. Jain, C. J. Moore, G. Ceder, Accuracy of density functional theory in predicting formation energies of ternary oxides from binary oxides and its implication on phase stability, Physical Review B, 85 (2012), 155208 ↩